# Electronic Supplementary Material (ESI) for Journal of Materials Chemistry A.
# This journal is © The Royal Society of Chemistry 2019

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_ZnPOM
_audit_block_doi                 10.5517/ccdc.csd.cc1m6g4f
_database_code_depnum_ccdc_archive 'CCDC 1495754'
loop_
_citation_id
_citation_doi
_citation_year
1 10.1021/acs.chemmater.7b00269 2017
_audit_update_record             
;
2016-07-23 deposited with the CCDC.
2019-01-18 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-2013
_chemical_name_systematic        
;
 ?
;
_chemical_name_common            ZnPOM
_chemical_melting_point          ?
_chemical_formula_moiety         'O88 W19.02 Zn8.98, 16(O), 4(H O), 14(Na)'
_chemical_formula_sum            'H4 Na14 O108 W19.02 Zn8.98'
_chemical_formula_weight         6138.21

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Zn Zn 0.2839 1.4301 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_H-M_alt        'P -1'
_space_group_name_Hall           '-P 1'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, -z'

_cell_length_a                   12.4391(4)
_cell_length_b                   13.6054(4)
_cell_length_c                   16.6803(6)
_cell_angle_alpha                82.3040(10)
_cell_angle_beta                 73.5230(10)
_cell_angle_gamma                64.2110(10)
_cell_volume                     2437.23(14)
_cell_formula_units_Z            1
_cell_measurement_temperature    100(2)
_cell_measurement_reflns_used    380
_cell_measurement_theta_min      2.20
_cell_measurement_theta_max      25.21

_exptl_crystal_description       'cylindrical rhombic'
_exptl_crystal_colour            colorless
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_density_diffrn    4.182
_exptl_crystal_F_000             2699
_exptl_transmission_factor_min   ?
_exptl_transmission_factor_max   ?
_exptl_crystal_size_max          0.320
_exptl_crystal_size_mid          0.210
_exptl_crystal_size_min          0.150
_exptl_absorpt_coefficient_mu    24.693
_shelx_estimated_absorpt_T_min   0.047
_shelx_estimated_absorpt_T_max   0.119
_exptl_absorpt_correction_type   empirical
_exptl_absorpt_correction_T_min  0.3892
_exptl_absorpt_correction_T_max  0.7457
_exptl_absorpt_process_details   SADABS

_exptl_special_details           
;
 ?
;

_diffrn_ambient_temperature      100(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_source                   'fine-focus microfocus tube'
_diffrn_measurement_device_type  'Bruker AXS CMOS-type PHOTON 100 detector'
_diffrn_measurement_method       omega-scans
_diffrn_detector_area_resol_mean ?
_diffrn_reflns_number            74766
_diffrn_reflns_av_unetI/netI     0.0263
_diffrn_reflns_av_R_equivalents  0.0380
_diffrn_reflns_limit_h_min       -16
_diffrn_reflns_limit_h_max       16
_diffrn_reflns_limit_k_min       -18
_diffrn_reflns_limit_k_max       18
_diffrn_reflns_limit_l_min       -22
_diffrn_reflns_limit_l_max       22
_diffrn_reflns_theta_min         2.522
_diffrn_reflns_theta_max         28.359
_diffrn_reflns_theta_full        25.242
_diffrn_measured_fraction_theta_max 0.997
_diffrn_measured_fraction_theta_full 0.999
_diffrn_reflns_Laue_measured_fraction_max 0.997
_diffrn_reflns_Laue_measured_fraction_full 0.999
_diffrn_reflns_point_group_measured_fraction_max 0.997
_diffrn_reflns_point_group_measured_fraction_full 0.999
_reflns_number_total             12166
_reflns_number_gt                11475
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_max     .
_reflns_Friedel_fraction_full    .

_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;

_computing_data_collection       'Bruker SMART'
_computing_cell_refinement       'Bruker SMART'
_computing_data_reduction        'Bruker SAINT'
_computing_structure_solution    SIR-97
_computing_structure_refinement  'SHELXL-2013 (Sheldrick, 2013)'
_computing_molecular_graphics    'DIAMOND 3'
_computing_publication_material  ?

_refine_special_details          
;
 ?
;
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0254P)²+47.7778P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   difmap
_refine_ls_hydrogen_treatment    constr
_refine_ls_extinction_method     SHELXL
_refine_ls_extinction_coef       0.000311(17)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_number_reflns         12166
_refine_ls_number_parameters     685
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0329
_refine_ls_R_factor_gt           0.0300
_refine_ls_wR_factor_ref         0.0742
_refine_ls_wR_factor_gt          0.0730
_refine_ls_goodness_of_fit_ref   1.151
_refine_ls_restrained_S_all      1.151
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
W1 W 0.07186(2) 0.10602(2) 0.10317(2) 0.00742(6) Uani 1 1 d . . . . .
W2 W 0.33862(2) -0.13518(2) 0.15966(2) 0.00822(6) Uani 1 1 d . . . . .
W3 W 0.29313(3) 0.14399(2) 0.19649(2) 0.00905(6) Uani 1 1 d . . . . .
W4 W -0.15991(2) 0.24473(2) 0.25762(2) 0.00795(6) Uani 1 1 d . . . . .
W5 W -0.11482(3) 0.00115(2) 0.22432(2) 0.00806(6) Uani 1 1 d . . . . .
W6 W 0.15227(3) -0.23743(2) 0.27694(2) 0.00960(7) Uani 1 1 d . . . . .
W7 W 0.34138(2) -0.19825(2) 0.35811(2) 0.00692(6) Uani 1 1 d . . . . .
W8 W 0.29051(2) 0.08719(2) 0.39482(2) 0.00735(6) Uani 1 1 d . . . . .
W9 W 0.06070(3) 0.29179(2) 0.34306(2) 0.00831(6) Uani 1 1 d . . . . .
Zn1 Zn 0.08528(7) 0.03058(6) 0.31933(5) 0.00588(15) Uani 1 1 d . . . . .
Zn2 Zn -0.02083(4) 0.12097(3) 0.51554(3) 0.00701(16) Uani 0.488(3) 1 d . . P A
1
W10 W -0.02083(4) 0.12097(3) 0.51554(3) 0.00701(16) Uani 0.512(3) 1 d . . P A 2
Zn3 Zn -0.20495(7) 0.08203(7) 0.43798(5) 0.01110(17) Uani 1 1 d . . . . .
Zn4 Zn 0.26448(10) 0.10989(9) -0.11505(6) 0.0203(2) Uani 1 1 d . . . . .
Zn5 Zn -0.39149(8) 0.47078(7) 0.16470(6) 0.01393(18) Uani 1 1 d . . . . .
Na1 Na 0.4145(7) 0.3726(6) 0.0591(4) 0.0762(19) Uani 1 1 d . . . . .
Na2 Na 0.6072(3) -0.4388(3) 0.4559(2) 0.0144(6) Uani 1 1 d . . . . .
Na3 Na 0.1473(15) 0.4167(11) -0.0591(11) 0.182(7) Uani 1 1 d . . . . .
Na4 Na 0.5356(7) 0.1942(6) 0.3136(4) 0.0735(19) Uani 1 1 d . . . . .
Na5 Na -0.3144(15) -0.1269(15) 0.3660(6) 0.183(7) Uani 1 1 d . . . . .
Na6 Na -0.0270(7) -0.3877(7) 0.4418(5) 0.079(2) Uani 1 1 d . . . . .
Na7 Na 0.1084(17) 0.717(2) 0.0707(11) 0.264(12) Uani 1 1 d . . . . .
O1 O -0.0129(4) 0.0881(4) 0.2387(3) 0.0075(9) Uani 1 1 d . . . . .
O2 O 0.2097(4) -0.1116(4) 0.2832(3) 0.0061(9) Uani 1 1 d . . . . .
O3 O 0.1687(4) 0.1223(4) 0.3123(3) 0.0074(9) Uani 1 1 d . . . . .
O4 O -0.0211(4) 0.0290(4) 0.4287(3) 0.0076(9) Uani 1 1 d . . . . .
O5 O 0.1228(5) 0.1220(4) -0.0038(3) 0.0114(10) Uani 1 1 d . . . . .
O6 O 0.4569(5) -0.1846(5) 0.0708(4) 0.0151(11) Uani 1 1 d . . . . .
O7 O 0.3964(5) 0.1783(5) 0.1164(4) 0.0149(11) Uani 1 1 d . . . . .
O8 O -0.0221(5) 0.0308(4) 0.1047(3) 0.0087(10) Uani 1 1 d . . . . .
O9 O -0.0589(5) 0.2401(4) 0.1312(3) 0.0101(10) Uani 1 1 d . . . . .
O10 O 0.2061(4) -0.0376(4) 0.1183(3) 0.0104(10) Uani 1 1 d . . . . .
O11 O 0.1770(5) 0.1581(5) 0.1392(3) 0.0125(10) Uani 1 1 d . . . . .
O12 O 0.2831(5) -0.2512(4) 0.1715(3) 0.0114(10) Uani 1 1 d . . . . .
O13 O 0.3625(5) -0.0098(4) 0.1796(3) 0.0125(10) Uani 1 1 d . . . . .
O14 O 0.4392(5) -0.2121(4) 0.2397(3) 0.0108(10) Uani 1 1 d . . . . .
O15 O 0.3833(5) 0.1123(5) 0.2818(4) 0.0158(11) Uani 1 1 d . . . . .
O16 O -0.1934(5) -0.0521(4) 0.1845(3) 0.0107(10) Uani 1 1 d . . . . .
O17 O -0.2222(5) 0.1562(4) 0.2175(3) 0.0098(10) Uani 1 1 d . . . . .
O18 O -0.2737(5) 0.3718(4) 0.2384(3) 0.0098(10) Uani 1 1 d . . . . .
O19 O -0.0455(5) 0.2949(4) 0.2795(4) 0.0139(11) Uani 1 1 d . . . . .
O20 O -0.2176(5) 0.2200(4) 0.3644(3) 0.0119(10) Uani 1 1 d . . . . .
O21 O 0.0335(5) -0.1308(4) 0.2260(4) 0.0125(11) Uani 1 1 d . . . . .
O22 O -0.1742(5) -0.0042(4) 0.3338(3) 0.0117(10) Uani 1 1 d . . . . .
O23 O 0.1371(5) -0.3541(4) 0.2638(4) 0.0169(12) Uani 1 1 d . . . . .
O24 O 0.2873(5) -0.3054(4) 0.3331(3) 0.0107(10) Uani 1 1 d . . . . .
O25 O 0.4600(5) -0.2920(5) 0.3989(4) 0.0161(11) Uani 1 1 d . . . . .
O26 O 0.3528(5) -0.0658(4) 0.3654(3) 0.0091(10) Uani 1 1 d . . . . .
O27 O 0.3960(6) 0.0747(5) 0.4483(4) 0.0187(12) Uani 1 1 d . . . . .
O28 O 0.1917(5) 0.2407(4) 0.4029(3) 0.0120(10) Uani 1 1 d . . . . .
O29 O 0.1887(5) 0.2914(4) 0.2411(3) 0.0122(10) Uani 1 1 d . . . . .
O30 O -0.0307(5) 0.2444(5) 0.4400(3) 0.0132(11) Uani 1 1 d . . . . .
O31 O 0.0053(6) 0.4278(4) 0.3635(4) 0.0179(12) Uani 1 1 d . . . . .
O32 O 0.2061(5) -0.1589(4) 0.4534(3) 0.0124(10) Uani 1 1 d . . . . .
O33 O 0.1666(5) 0.0638(4) 0.4821(3) 0.0136(11) Uani 1 1 d . . . . .
O34 O 0.0450(5) -0.1944(5) 0.3856(4) 0.0149(11) Uani 1 1 d . . . . .
O35 O 0.3072(12) 0.2014(12) -0.0414(8) 0.020(3) Uani 0.5 1 d . . P B 1
O35A O 0.358(2) 0.127(2) -0.0367(12) 0.067(7) Uani 0.5 1 d . . P B 2
O36 O 0.3586(7) -0.0478(10) -0.0813(7) 0.081(4) Uani 1 1 d . . . . .
O37 O 0.3965(7) 0.1113(8) -0.2248(4) 0.039(2) Uani 1 1 d . . . . .
O38 O 0.1422(16) 0.2687(8) -0.1401(6) 0.101(6) Uani 1 1 d . . . . .
O39 O -0.2267(7) 0.4315(7) 0.0663(4) 0.040(2) Uani 1 1 d . . . . .
O40 O -0.4096(7) 0.3348(5) 0.1390(5) 0.0325(17) Uani 1 1 d . . . . .
O41 O -0.5409(5) 0.4979(5) 0.2735(4) 0.0157(11) Uani 1 1 d . . . . .
O42 O -0.3622(5) 0.5990(5) 0.1964(4) 0.0179(12) Uani 1 1 d . . . . .
O43 O -0.5115(5) 0.5665(4) 0.0939(4) 0.0163(11) Uani 1 1 d . . . . .
O44 O 0.1849(12) 0.5163(14) 0.1333(13) 0.136(8) Uani 1 1 d . . . . .
O45 O -0.3909(5) 0.1259(5) 0.4573(4) 0.0166(11) Uani 1 1 d . . . . .
O46 O 0.5567(5) -0.5802(5) 0.4206(4) 0.0161(11) Uani 1 1 d . . . . .
O47 O 0.6563(7) -0.3080(7) 0.5037(7) 0.053(3) Uani 1 1 d . . . . .
O48 O 0.7602(5) -0.5672(5) 0.5244(4) 0.0200(13) Uani 1 1 d . . . . .
O49 O 0.7574(5) -0.4604(5) 0.3223(4) 0.0191(12) Uani 1 1 d . . . . .
O50 O 0.1659(6) -0.5666(5) 0.4464(4) 0.0211(12) Uani 1 1 d . . . . .
H50 H 0.2030 -0.6018 0.4465 0.025 Uiso 1 1 d R U . . .
O51 O -0.1314(14) -0.3179(10) 0.2948(9) 0.100(6) Uani 1 1 d . . . . .
O52 O -0.2081(11) 0.1566(7) 0.0220(7) 0.066(3) Uani 1 1 d . . . . .
O53 O 0.035(2) 0.4246(12) 0.1133(12) 0.135(8) Uani 1 1 d . . . . .
O54 O 0.3068(16) 0.3983(14) 0.3039(6) 0.117(7) Uani 1 1 d . . . . .
H54 H 0.2611 0.4405 0.2997 0.141 Uiso 1 1 d R U . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
W1 O5 1.734(5) . ?
W1 O9 1.846(5) . ?
W1 O8 1.852(5) . ?
W1 O10 1.985(5) . ?
W1 O11 1.985(5) . ?
W1 O1 2.238(5) . ?
W2 O6 1.727(5) . ?
W2 O10 1.858(5) . ?
W2 O13 1.938(5) . ?
W2 O12 1.947(5) . ?
W2 O14 1.969(5) . ?
W2 O2 2.186(5) . ?
W3 O7 1.742(5) . ?
W3 O11 1.878(5) . ?
W3 O13 1.911(5) . ?
W3 O15 1.946(6) . ?
W3 O29 1.962(5) . ?
W3 O3 2.183(5) . ?
W4 O18 1.753(5) . ?
W4 O20 1.768(5) . ?
W4 O17 1.955(5) . ?
W4 O19 1.957(5) . ?
W4 O1 2.109(5) . ?
W4 O9 2.120(5) . ?
W4 W5 3.2101(4) . ?
W5 O16 1.742(5) . ?
W5 O22 1.770(5) . ?
W5 O21 1.940(5) . ?
W5 O17 1.954(5) . ?
W5 O8 2.087(5) . ?
W5 O1 2.149(5) . ?
W6 O23 1.727(5) . ?
W6 O21 1.878(5) . ?
W6 O34 1.908(6) . ?
W6 O24 1.965(5) . ?
W6 O12 1.994(5) . ?
W6 O2 2.147(5) . ?
W7 O25 1.723(5) . ?
W7 O32 1.890(5) . ?
W7 O26 1.890(5) . ?
W7 O24 1.982(5) . ?
W7 O14 1.989(5) . ?
W7 O2 2.172(5) . ?
W8 O27 1.726(5) . ?
W8 O33 1.904(6) . ?
W8 O28 1.908(5) . ?
W8 O26 1.957(5) . ?
W8 O15 1.986(6) . ?
W8 O3 2.190(5) . ?
W9 O31 1.715(5) . ?
W9 O19 1.899(5) . ?
W9 O30 1.907(5) . ?
W9 O28 1.971(5) . ?
W9 O29 1.972(5) . ?
W9 O3 2.148(5) . ?
Zn1 O3 1.915(5) . ?
Zn1 O2 1.918(5) . ?
Zn1 O4 1.930(5) . ?
Zn1 O1 1.931(5) . ?
Zn2 O34 1.926(6) 2_556 ?
Zn2 O30 1.940(6) . ?
Zn2 O4 2.035(5) 2_556 ?
Zn2 O33 2.038(6) . ?
Zn2 O4 2.039(5) . ?
Zn2 O32 2.051(5) 2_556 ?
Zn3 O4 2.042(5) . ?
Zn3 O45 2.059(6) . ?
Zn3 O20 2.071(6) . ?
Zn3 O22 2.078(5) . ?
Zn3 O33 2.184(6) 2_556 ?
Zn3 O32 2.204(6) 2_556 ?
Zn3 W10 3.1669(10) 2_556 ?
Zn4 O36 2.038(10) . ?
Zn4 O16 2.043(5) 2 ?
Zn4 O35A 2.070(19) . ?
Zn4 O37 2.089(7) . ?
Zn4 O38 2.101(12) . ?
Zn4 O5 2.134(5) . ?
Zn4 O35 2.168(14) . ?
Zn5 O43 2.053(6) . ?
Zn5 O40 2.070(7) . ?
Zn5 O18 2.082(5) . ?
Zn5 O42 2.089(6) . ?
Zn5 O39 2.134(7) . ?
Zn5 O41 2.134(6) . ?
Na1 O43 2.686(9) 2_565 ?
Na1 O44 2.701(15) . ?
Na1 O40 2.705(11) 1_655 ?
Na1 O7 2.769(9) . ?
Na1 Na3 4.118(16) . ?
Na2 O25 2.354(6) . ?
Na2 O46 2.402(6) 2_646 ?
Na2 O47 2.402(8) . ?
Na2 O48 2.405(7) . ?
Na2 O49 2.425(7) . ?
Na2 O46 2.452(7) . ?
Na2 Na2 3.610(6) 2_646 ?
Na3 O38 2.603(18) . ?
Na3 O39 2.625(14) 2_565 ?
Na3 O53 2.64(2) 2_565 ?
Na3 O35 2.77(2) . ?
Na3 O53 2.81(3) . ?
Na3 O42 2.932(19) 2_565 ?
Na3 Na3 3.51(4) 2_565 ?
Na4 O45 2.712(9) 1_655 ?
Na4 O15 2.770(8) . ?
Na4 O17 2.836(9) 1_655 ?
Na4 O54 3.02(2) . ?
Na4 Na5 4.017(19) 1_655 ?
Na5 O51 2.74(2) . ?
Na5 O37 2.770(12) 2 ?
Na5 O22 2.807(11) . ?
Na5 Na4 4.017(19) 1_455 ?
Na5 Na6 4.16(2) . ?
Na6 O50 2.376(9) 2_546 ?
Na6 O50 2.580(11) . ?
Na6 O31 2.805(9) 1_545 ?
Na6 O51 2.951(13) . ?
Na6 Na6 3.305(16) 2_546 ?
Na7 O52 2.63(2) 2_565 ?
Na7 O44 2.65(3) . ?
Na7 O39 2.87(3) 2_565 ?
Na7 O38 2.93(2) 2_565 ?
O4 W10 2.035(5) 2_556 ?
O4 Zn2 2.035(5) 2_556 ?
O16 Zn4 2.043(5) 2 ?
O17 Na4 2.836(9) 1_455 ?
O31 Na6 2.805(9) 1_565 ?
O32 W10 2.051(5) 2_556 ?
O32 Zn2 2.051(5) 2_556 ?
O32 Zn3 2.204(6) 2_556 ?
O33 Zn3 2.184(6) 2_556 ?
O34 W10 1.926(6) 2_556 ?
O34 Zn2 1.926(6) 2_556 ?
O37 Na5 2.770(12) 2 ?
O38 Na7 2.93(2) 2_565 ?
O39 Na3 2.625(14) 2_565 ?
O39 Na7 2.87(3) 2_565 ?
O40 Na1 2.705(11) 1_455 ?
O42 Na3 2.932(19) 2_565 ?
O43 Na1 2.686(9) 2_565 ?
O45 Na4 2.712(9) 1_455 ?
O46 Na2 2.402(6) 2_646 ?
O50 Na6 2.376(9) 2_546 ?
O50 H50 0.4998 . ?
O52 Na7 2.63(2) 2_565 ?
O53 Na3 2.64(2) 2_565 ?
O54 H54 0.6204 . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O5 W1 O9 101.4(2) . . ?
O5 W1 O8 100.0(2) . . ?
O9 W1 O8 96.4(2) . . ?
O5 W1 O10 98.8(2) . . ?
O9 W1 O10 158.6(2) . . ?
O8 W1 O10 87.0(2) . . ?
O5 W1 O11 98.0(2) . . ?
O9 W1 O11 88.9(2) . . ?
O8 W1 O11 159.8(2) . . ?
O10 W1 O11 81.3(2) . . ?
O5 W1 O1 173.9(2) . . ?
O9 W1 O1 75.7(2) . . ?
O8 W1 O1 75.1(2) . . ?
O10 W1 O1 84.83(19) . . ?
O11 W1 O1 87.5(2) . . ?
O6 W2 O10 103.7(2) . . ?
O6 W2 O13 99.5(2) . . ?
O10 W2 O13 87.1(2) . . ?
O6 W2 O12 96.6(2) . . ?
O10 W2 O12 92.2(2) . . ?
O13 W2 O12 163.6(2) . . ?
O6 W2 O14 95.9(2) . . ?
O10 W2 O14 159.9(2) . . ?
O13 W2 O14 85.3(2) . . ?
O12 W2 O14 89.9(2) . . ?
O6 W2 O2 166.5(2) . . ?
O10 W2 O2 87.5(2) . . ?
O13 W2 O2 88.4(2) . . ?
O12 W2 O2 75.2(2) . . ?
O14 W2 O2 73.71(19) . . ?
O7 W3 O11 100.0(3) . . ?
O7 W3 O13 99.7(2) . . ?
O11 W3 O13 87.6(2) . . ?
O7 W3 O15 97.0(2) . . ?
O11 W3 O15 162.8(2) . . ?
O13 W3 O15 87.5(2) . . ?
O7 W3 O29 97.0(2) . . ?
O11 W3 O29 90.1(2) . . ?
O13 W3 O29 163.3(2) . . ?
O15 W3 O29 89.8(2) . . ?
O7 W3 O3 168.2(2) . . ?
O11 W3 O3 88.6(2) . . ?
O13 W3 O3 88.6(2) . . ?
O15 W3 O3 74.9(2) . . ?
O29 W3 O3 74.8(2) . . ?
O18 W4 O20 102.9(2) . . ?
O18 W4 O17 96.3(2) . . ?
O20 W4 O17 94.2(2) . . ?
O18 W4 O19 98.8(2) . . ?
O20 W4 O19 93.8(2) . . ?
O17 W4 O19 160.9(2) . . ?
O18 W4 O1 161.4(2) . . ?
O20 W4 O1 94.1(2) . . ?
O17 W4 O1 74.7(2) . . ?
O19 W4 O1 87.4(2) . . ?
O18 W4 O9 89.7(2) . . ?
O20 W4 O9 167.4(2) . . ?
O17 W4 O9 83.8(2) . . ?
O19 W4 O9 84.6(2) . . ?
O1 W4 O9 73.4(2) . . ?
O18 W4 W5 131.05(17) . . ?
O20 W4 W5 86.89(18) . . ?
O17 W4 W5 34.77(15) . . ?
O19 W4 W5 128.73(16) . . ?
O1 W4 W5 41.55(13) . . ?
O9 W4 W5 84.41(14) . . ?
O16 W5 O22 103.4(2) . . ?
O16 W5 O21 99.1(2) . . ?
O22 W5 O21 92.5(2) . . ?
O16 W5 O17 98.7(2) . . ?
O22 W5 O17 92.7(2) . . ?
O21 W5 O17 159.7(2) . . ?
O16 W5 O8 92.2(2) . . ?
O22 W5 O8 164.3(2) . . ?
O21 W5 O8 86.9(2) . . ?
O17 W5 O8 82.8(2) . . ?
O16 W5 O1 163.7(2) . . ?
O22 W5 O1 91.6(2) . . ?
O21 W5 O1 86.4(2) . . ?
O17 W5 O1 73.8(2) . . ?
O8 W5 O1 72.69(19) . . ?
O16 W5 W4 133.53(18) . . ?
O22 W5 W4 84.55(18) . . ?
O21 W5 W4 126.53(15) . . ?
O17 W5 W4 34.80(15) . . ?
O8 W5 W4 83.23(14) . . ?
O1 W5 W4 40.59(13) . . ?
O23 W6 O21 101.8(2) . . ?
O23 W6 O34 100.8(3) . . ?
O21 W6 O34 91.4(2) . . ?
O23 W6 O24 97.9(2) . . ?
O21 W6 O24 160.3(2) . . ?
O34 W6 O24 86.4(2) . . ?
O23 W6 O12 96.0(3) . . ?
O21 W6 O12 90.2(2) . . ?
O34 W6 O12 162.4(2) . . ?
O24 W6 O12 86.2(2) . . ?
O23 W6 O2 168.5(2) . . ?
O21 W6 O2 85.8(2) . . ?
O34 W6 O2 87.5(2) . . ?
O24 W6 O2 74.6(2) . . ?
O12 W6 O2 75.1(2) . . ?
O25 W7 O32 102.3(3) . . ?
O25 W7 O26 102.6(2) . . ?
O32 W7 O26 89.5(2) . . ?
O25 W7 O24 95.8(2) . . ?
O32 W7 O24 87.6(2) . . ?
O26 W7 O24 161.6(2) . . ?
O25 W7 O14 96.3(2) . . ?
O32 W7 O14 161.2(2) . . ?
O26 W7 O14 89.7(2) . . ?
O24 W7 O14 87.2(2) . . ?
O25 W7 O2 165.5(2) . . ?
O32 W7 O2 87.5(2) . . ?
O26 W7 O2 88.0(2) . . ?
O24 W7 O2 73.70(19) . . ?
O14 W7 O2 73.63(19) . . ?
O27 W8 O33 101.5(3) . . ?
O27 W8 O28 100.1(3) . . ?
O33 W8 O28 89.5(2) . . ?
O27 W8 O26 99.2(3) . . ?
O33 W8 O26 87.0(2) . . ?
O28 W8 O26 160.7(2) . . ?
O27 W8 O15 97.4(3) . . ?
O33 W8 O15 161.0(2) . . ?
O28 W8 O15 88.7(2) . . ?
O26 W8 O15 88.4(2) . . ?
O27 W8 O3 169.9(2) . . ?
O33 W8 O3 87.3(2) . . ?
O28 W8 O3 74.9(2) . . ?
O26 W8 O3 86.0(2) . . ?
O15 W8 O3 74.0(2) . . ?
O31 W9 O19 101.2(3) . . ?
O31 W9 O30 101.2(3) . . ?
O19 W9 O30 90.8(2) . . ?
O31 W9 O28 96.3(2) . . ?
O19 W9 O28 162.5(2) . . ?
O30 W9 O28 85.6(2) . . ?
O31 W9 O29 95.7(3) . . ?
O19 W9 O29 91.8(2) . . ?
O30 W9 O29 162.0(2) . . ?
O28 W9 O29 86.5(2) . . ?
O31 W9 O3 167.5(2) . . ?
O19 W9 O3 88.1(2) . . ?
O30 W9 O3 86.9(2) . . ?
O28 W9 O3 74.6(2) . . ?
O29 W9 O3 75.4(2) . . ?
O3 Zn1 O2 106.9(2) . . ?
O3 Zn1 O4 113.2(2) . . ?
O2 Zn1 O4 113.1(2) . . ?
O3 Zn1 O1 106.3(2) . . ?
O2 Zn1 O1 107.9(2) . . ?
O4 Zn1 O1 109.2(2) . . ?
O34 Zn2 O30 95.9(2) 2_556 . ?
O34 Zn2 O4 94.8(2) 2_556 2_556 ?
O30 Zn2 O4 166.4(2) . 2_556 ?
O34 Zn2 O33 95.7(2) 2_556 . ?
O30 Zn2 O33 89.3(2) . . ?
O4 Zn2 O33 81.3(2) 2_556 . ?
O34 Zn2 O4 167.0(2) 2_556 . ?
O30 Zn2 O4 94.0(2) . . ?
O4 Zn2 O4 76.8(2) 2_556 . ?
O33 Zn2 O4 92.9(2) . . ?
O34 Zn2 O32 89.2(2) 2_556 2_556 ?
O30 Zn2 O32 95.5(2) . 2_556 ?
O4 Zn2 O32 93.0(2) 2_556 2_556 ?
O33 Zn2 O32 172.8(2) . 2_556 ?
O4 Zn2 O32 81.4(2) . 2_556 ?
O4 Zn3 O45 174.5(2) . . ?
O4 Zn3 O20 94.3(2) . . ?
O45 Zn3 O20 90.9(2) . . ?
O4 Zn3 O22 93.4(2) . . ?
O45 Zn3 O22 88.4(2) . . ?
O20 Zn3 O22 90.5(2) . . ?
O4 Zn3 O33 77.7(2) . 2_556 ?
O45 Zn3 O33 97.0(2) . 2_556 ?
O20 Zn3 O33 171.6(2) . 2_556 ?
O22 Zn3 O33 92.7(2) . 2_556 ?
O4 Zn3 O32 77.7(2) . 2_556 ?
O45 Zn3 O32 100.3(2) . 2_556 ?
O20 Zn3 O32 91.7(2) . 2_556 ?
O22 Zn3 O32 170.9(2) . 2_556 ?
O33 Zn3 O32 83.9(2) 2_556 2_556 ?
O4 Zn3 W10 38.94(14) . 2_556 ?
O45 Zn3 W10 136.06(17) . 2_556 ?
O20 Zn3 W10 132.83(15) . 2_556 ?
O22 Zn3 W10 87.42(15) . 2_556 ?
O33 Zn3 W10 39.69(15) 2_556 2_556 ?
O32 Zn3 W10 84.65(14) 2_556 2_556 ?
O36 Zn4 O16 87.7(4) . 2 ?
O36 Zn4 O35A 77.6(9) . . ?
O16 Zn4 O35A 165.3(9) 2 . ?
O36 Zn4 O37 96.6(4) . . ?
O16 Zn4 O37 87.4(2) 2 . ?
O35A Zn4 O37 94.7(5) . . ?
O36 Zn4 O38 170.9(5) . . ?
O16 Zn4 O38 88.2(4) 2 . ?
O35A Zn4 O38 106.2(9) . . ?
O37 Zn4 O38 91.2(4) . . ?
O36 Zn4 O5 87.7(3) . . ?
O16 Zn4 O5 93.8(2) 2 . ?
O35A Zn4 O5 85.2(5) . . ?
O37 Zn4 O5 175.5(3) . . ?
O38 Zn4 O5 84.5(4) . . ?
O36 Zn4 O35 102.8(6) . . ?
O16 Zn4 O35 168.5(4) 2 . ?
O37 Zn4 O35 95.9(4) . . ?
O38 Zn4 O35 80.7(6) . . ?
O5 Zn4 O35 82.1(4) . . ?
O43 Zn5 O40 90.3(3) . . ?
O43 Zn5 O18 178.2(2) . . ?
O40 Zn5 O18 88.6(2) . . ?
O43 Zn5 O42 94.7(2) . . ?
O40 Zn5 O42 175.0(3) . . ?
O18 Zn5 O42 86.4(2) . . ?
O43 Zn5 O39 96.6(3) . . ?
O40 Zn5 O39 91.0(3) . . ?
O18 Zn5 O39 84.8(2) . . ?
O42 Zn5 O39 88.2(3) . . ?
O43 Zn5 O41 90.9(2) . . ?
O40 Zn5 O41 89.3(3) . . ?
O18 Zn5 O41 87.7(2) . . ?
O42 Zn5 O41 90.9(2) . . ?
O39 Zn5 O41 172.5(3) . . ?
O43 Na1 O44 114.7(6) 2_565 . ?
O43 Na1 O40 101.7(3) 2_565 1_655 ?
O44 Na1 O40 115.6(4) . 1_655 ?
O43 Na1 O7 130.9(3) 2_565 . ?
O44 Na1 O7 99.9(5) . . ?
O40 Na1 O7 92.7(3) 1_655 . ?
O43 Na1 Na3 79.9(3) 2_565 . ?
O44 Na1 Na3 65.2(4) . . ?
O40 Na1 Na3 177.5(3) 1_655 . ?
O7 Na1 Na3 84.8(3) . . ?
O25 Na2 O46 86.9(2) . 2_646 ?
O25 Na2 O47 88.0(3) . . ?
O46 Na2 O47 92.3(3) 2_646 . ?
O25 Na2 O48 171.0(3) . . ?
O46 Na2 O48 92.0(2) 2_646 . ?
O47 Na2 O48 83.2(3) . . ?
O25 Na2 O49 89.3(2) . . ?
O46 Na2 O49 173.2(2) 2_646 . ?
O47 Na2 O49 93.1(3) . . ?
O48 Na2 O49 92.6(2) . . ?
O25 Na2 O46 95.8(2) . . ?
O46 Na2 O46 83.9(2) 2_646 . ?
O47 Na2 O46 174.5(3) . . ?
O48 Na2 O46 92.9(2) . . ?
O49 Na2 O46 90.9(2) . . ?
O25 Na2 Na2 91.83(19) . 2_646 ?
O46 Na2 Na2 42.48(16) 2_646 2_646 ?
O47 Na2 Na2 134.7(3) . 2_646 ?
O48 Na2 Na2 93.35(19) . 2_646 ?
O49 Na2 Na2 132.2(2) . 2_646 ?
O46 Na2 Na2 41.41(15) . 2_646 ?
O38 Na3 O39 146.5(8) . 2_565 ?
O38 Na3 O53 92.7(6) . 2_565 ?
O39 Na3 O53 83.6(5) 2_565 2_565 ?
O38 Na3 O35 61.9(5) . . ?
O39 Na3 O35 118.3(6) 2_565 . ?
O53 Na3 O35 154.5(7) 2_565 . ?
O38 Na3 O53 115.0(5) . . ?
O39 Na3 O53 98.4(6) 2_565 . ?
O53 Na3 O53 100.0(7) 2_565 . ?
O35 Na3 O53 90.0(6) . . ?
O38 Na3 O42 84.8(6) . 2_565 ?
O39 Na3 O42 63.6(4) 2_565 2_565 ?
O53 Na3 O42 101.7(7) 2_565 2_565 ?
O35 Na3 O42 79.4(6) . 2_565 ?
O53 Na3 O42 149.8(6) . 2_565 ?
O38 Na3 Na3 112.0(7) . 2_565 ?
O39 Na3 Na3 92.0(6) 2_565 2_565 ?
O53 Na3 Na3 52.1(6) 2_565 2_565 ?
O35 Na3 Na3 132.7(7) . 2_565 ?
O53 Na3 Na3 47.9(6) . 2_565 ?
O42 Na3 Na3 147.6(6) 2_565 2_565 ?
O38 Na3 Na1 125.9(6) . . ?
O39 Na3 Na1 59.3(3) 2_565 . ?
O53 Na3 Na1 140.2(5) 2_565 . ?
O35 Na3 Na1 65.1(4) . . ?
O53 Na3 Na1 74.1(5) . . ?
O42 Na3 Na1 75.9(3) 2_565 . ?
Na3 Na3 Na1 111.0(6) 2_565 . ?
O45 Na4 O15 116.6(3) 1_655 . ?
O45 Na4 O17 92.7(3) 1_655 1_655 ?
O15 Na4 O17 126.1(3) . 1_655 ?
O45 Na4 O54 122.4(4) 1_655 . ?
O15 Na4 O54 77.4(3) . . ?
O17 Na4 O54 124.9(3) 1_655 . ?
O45 Na4 Na5 60.6(2) 1_655 1_655 ?
O15 Na4 Na5 74.4(2) . 1_655 ?
O17 Na4 Na5 84.4(3) 1_655 1_655 ?
O54 Na4 Na5 148.1(3) . 1_655 ?
O51 Na5 O37 83.2(4) . 2 ?
O51 Na5 O22 97.9(5) . . ?
O37 Na5 O22 107.2(4) 2 . ?
O51 Na5 Na4 140.3(4) . 1_455 ?
O37 Na5 Na4 75.1(4) 2 1_455 ?
O22 Na5 Na4 59.0(3) . 1_455 ?
O51 Na5 Na6 45.1(4) . . ?
O37 Na5 Na6 127.9(6) 2 . ?
O22 Na5 Na6 89.2(4) . . ?
Na4 Na5 Na6 147.0(3) 1_455 . ?
O50 Na6 O50 96.5(3) 2_546 . ?
O50 Na6 O31 85.4(3) 2_546 1_545 ?
O50 Na6 O31 61.6(2) . 1_545 ?
O50 Na6 O51 109.4(4) 2_546 . ?
O50 Na6 O51 122.9(4) . . ?
O31 Na6 O51 70.7(3) 1_545 . ?
O50 Na6 Na6 50.9(3) 2_546 2_546 ?
O50 Na6 Na6 45.6(2) . 2_546 ?
O31 Na6 Na6 64.5(3) 1_545 2_546 ?
O51 Na6 Na6 131.5(4) . 2_546 ?
O50 Na6 Na5 92.1(3) 2_546 . ?
O50 Na6 Na5 163.9(3) . . ?
O31 Na6 Na5 105.8(3) 1_545 . ?
O51 Na6 Na5 41.0(4) . . ?
Na6 Na6 Na5 141.0(4) 2_546 . ?
O52 Na7 O44 137.5(9) 2_565 . ?
O52 Na7 O39 87.5(6) 2_565 2_565 ?
O44 Na7 O39 72.2(8) . 2_565 ?
O52 Na7 O38 136.0(10) 2_565 2_565 ?
O44 Na7 O38 86.4(7) . 2_565 ?
O39 Na7 O38 108.2(7) 2_565 2_565 ?
Zn1 O1 W4 118.8(2) . . ?
Zn1 O1 W5 117.2(2) . . ?
W4 O1 W5 97.86(19) . . ?
Zn1 O1 W1 121.7(2) . . ?
W4 O1 W1 98.6(2) . . ?
W5 O1 W1 98.0(2) . . ?
Zn1 O2 W6 118.4(2) . . ?
Zn1 O2 W7 117.6(2) . . ?
W6 O2 W7 98.7(2) . . ?
Zn1 O2 W2 121.0(2) . . ?
W6 O2 W2 97.68(19) . . ?
W7 O2 W2 98.96(19) . . ?
Zn1 O3 W9 118.8(2) . . ?
Zn1 O3 W3 122.2(3) . . ?
W9 O3 W3 97.7(2) . . ?
Zn1 O3 W8 118.7(2) . . ?
W9 O3 W8 96.7(2) . . ?
W3 O3 W8 97.58(19) . . ?
Zn1 O4 W10 114.7(2) . 2_556 ?
Zn1 O4 Zn2 114.7(2) . 2_556 ?
Zn1 O4 Zn2 114.8(2) . . ?
Zn2 O4 Zn2 103.2(2) 2_556 . ?
Zn1 O4 Zn3 117.7(2) . . ?
W10 O4 Zn3 101.9(2) 2_556 . ?
Zn2 O4 Zn3 101.9(2) 2_556 . ?
Zn2 O4 Zn3 102.4(2) . . ?
W1 O5 Zn4 152.2(3) . . ?
W3 O7 Na1 134.1(3) . . ?
W1 O8 W5 114.2(2) . . ?
W1 O9 W4 112.3(2) . . ?
W2 O10 W1 156.2(3) . . ?
W3 O11 W1 153.6(3) . . ?
W2 O12 W6 111.7(3) . . ?
W3 O13 W2 147.9(3) . . ?
W2 O14 W7 113.7(2) . . ?
W3 O15 W8 113.6(2) . . ?
W3 O15 Na4 133.4(3) . . ?
W8 O15 Na4 103.8(3) . . ?
W5 O16 Zn4 168.5(3) . 2 ?
W5 O17 W4 110.4(2) . . ?
W5 O17 Na4 109.0(3) . 1_455 ?
W4 O17 Na4 110.7(3) . 1_455 ?
W4 O18 Zn5 149.6(3) . . ?
W9 O19 W4 151.5(3) . . ?
W4 O20 Zn3 135.1(3) . . ?
W6 O21 W5 154.3(3) . . ?
W5 O22 Zn3 137.5(3) . . ?
W5 O22 Na5 108.2(3) . . ?
Zn3 O22 Na5 112.1(3) . . ?
W6 O24 W7 112.3(2) . . ?
W7 O25 Na2 171.0(3) . . ?
W7 O26 W8 155.6(3) . . ?
W8 O28 W9 113.3(3) . . ?
W3 O29 W9 112.0(2) . . ?
W9 O30 Zn2 143.0(3) . . ?
W9 O31 Na6 157.2(4) . 1_565 ?
W7 O32 W10 139.0(3) . 2_556 ?
W7 O32 Zn2 139.0(3) . 2_556 ?
W7 O32 Zn3 121.5(3) . 2_556 ?
W10 O32 Zn3 96.7(2) 2_556 2_556 ?
Zn2 O32 Zn3 96.7(2) 2_556 2_556 ?
W8 O33 Zn2 137.9(3) . . ?
W8 O33 Zn3 123.1(3) . 2_556 ?
Zn2 O33 Zn3 97.1(2) . 2_556 ?
W6 O34 W10 142.4(3) . 2_556 ?
W6 O34 Zn2 142.4(3) . 2_556 ?
Zn4 O35 Na3 104.7(6) . . ?
Zn4 O37 Na5 111.9(4) . 2 ?
Zn4 O38 Na3 112.6(7) . . ?
Zn4 O38 Na7 107.1(7) . 2_565 ?
Na3 O38 Na7 103.6(7) . 2_565 ?
Zn5 O39 Na3 108.3(5) . 2_565 ?
Zn5 O39 Na7 134.6(5) . 2_565 ?
Na3 O39 Na7 115.8(6) 2_565 2_565 ?
Zn5 O40 Na1 116.2(3) . 1_455 ?
Zn5 O42 Na3 99.4(3) . 2_565 ?
Zn5 O43 Na1 117.4(3) . 2_565 ?
Na7 O44 Na1 117.1(9) . . ?
Zn3 O45 Na4 111.7(3) . 1_455 ?
Na2 O46 Na2 96.1(2) 2_646 . ?
Na6 O50 Na6 83.5(3) 2_546 . ?
Na6 O50 H50 96.8 2_546 . ?
Na6 O50 H50 178.1 . . ?
Na5 O51 Na6 93.9(5) . . ?
Na3 O53 Na3 80.0(7) 2_565 . ?
Na4 O54 H54 176.7 . . ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
O9 W1 O5 Zn4 132.0(6) . . . . ?
O8 W1 O5 Zn4 -129.3(6) . . . . ?
O10 W1 O5 Zn4 -40.8(7) . . . . ?
O11 W1 O5 Zn4 41.5(7) . . . . ?
O11 W3 O7 Na1 89.2(5) . . . . ?
O13 W3 O7 Na1 178.5(4) . . . . ?
O15 W3 O7 Na1 -92.9(5) . . . . ?
O29 W3 O7 Na1 -2.2(5) . . . . ?
O3 W3 O7 Na1 -47.2(13) . . . . ?
O5 W1 O8 W5 -176.0(3) . . . . ?
O9 W1 O8 W5 -73.2(3) . . . . ?
O10 W1 O8 W5 85.6(3) . . . . ?
O11 W1 O8 W5 31.3(8) . . . . ?
O1 W1 O8 W5 0.1(2) . . . . ?
O5 W1 O9 W4 173.0(3) . . . . ?
O8 W1 O9 W4 71.3(3) . . . . ?
O10 W1 O9 W4 -26.9(7) . . . . ?
O11 W1 O9 W4 -89.1(3) . . . . ?
O1 W1 O9 W4 -1.5(2) . . . . ?
O6 W2 O10 W1 -120.6(7) . . . . ?
O13 W2 O10 W1 -21.6(7) . . . . ?
O12 W2 O10 W1 142.0(7) . . . . ?
O14 W2 O10 W1 46.4(12) . . . . ?
O2 W2 O10 W1 67.0(7) . . . . ?
O7 W3 O11 W1 129.6(7) . . . . ?
O13 W3 O11 W1 30.2(7) . . . . ?
O15 W3 O11 W1 -43.4(13) . . . . ?
O29 W3 O11 W1 -133.3(7) . . . . ?
O3 W3 O11 W1 -58.5(7) . . . . ?
O22 W5 O16 Zn4 -178.5(16) . . . 2 ?
O21 W5 O16 Zn4 -83.7(17) . . . 2 ?
O17 W5 O16 Zn4 86.6(17) . . . 2 ?
O8 W5 O16 Zn4 3.6(17) . . . 2 ?
O1 W5 O16 Zn4 25(2) . . . 2 ?
W4 W5 O16 Zn4 86.3(17) . . . 2 ?
O20 W4 O18 Zn5 -131.5(6) . . . . ?
O17 W4 O18 Zn5 -35.8(6) . . . . ?
O19 W4 O18 Zn5 132.5(6) . . . . ?
O1 W4 O18 Zn5 24.0(11) . . . . ?
O9 W4 O18 Zn5 48.0(6) . . . . ?
W5 W4 O18 Zn5 -34.3(7) . . . . ?
O31 W9 O19 W4 -127.8(6) . . . . ?
O30 W9 O19 W4 -26.3(7) . . . . ?
O28 W9 O19 W4 51.8(12) . . . . ?
O29 W9 O19 W4 135.9(6) . . . . ?
O3 W9 O19 W4 60.6(6) . . . . ?
O18 W4 O20 Zn3 149.6(4) . . . . ?
O17 W4 O20 Zn3 52.1(4) . . . . ?
O19 W4 O20 Zn3 -110.5(4) . . . . ?
O1 W4 O20 Zn3 -22.8(4) . . . . ?
O9 W4 O20 Zn3 -28.3(13) . . . . ?
W5 W4 O20 Zn3 18.1(4) . . . . ?
O23 W6 O21 W5 118.9(7) . . . . ?
O34 W6 O21 W5 17.5(7) . . . . ?
O24 W6 O21 W5 -65.7(11) . . . . ?
O12 W6 O21 W5 -145.0(7) . . . . ?
O2 W6 O21 W5 -69.9(7) . . . . ?
O16 W5 O22 Zn3 -150.7(4) . . . . ?
O21 W5 O22 Zn3 109.3(4) . . . . ?
O17 W5 O22 Zn3 -51.0(4) . . . . ?
O8 W5 O22 Zn3 21.7(11) . . . . ?
O1 W5 O22 Zn3 22.9(4) . . . . ?
W4 W5 O22 Zn3 -17.1(4) . . . . ?
O16 W5 O22 Na5 10.3(5) . . . . ?
O21 W5 O22 Na5 -89.7(5) . . . . ?
O17 W5 O22 Na5 109.9(5) . . . . ?
O8 W5 O22 Na5 -177.4(8) . . . . ?
O1 W5 O22 Na5 -176.2(5) . . . . ?
W4 W5 O22 Na5 143.8(5) . . . . ?
O25 W7 O26 W8 -129.8(7) . . . . ?
O32 W7 O26 W8 -27.3(7) . . . . ?
O24 W7 O26 W8 53.6(12) . . . . ?
O14 W7 O26 W8 133.8(7) . . . . ?
O2 W7 O26 W8 60.2(7) . . . . ?
O19 W9 O31 Na6 165.8(9) . . . 1_565 ?
O30 W9 O31 Na6 72.7(10) . . . 1_565 ?
O28 W9 O31 Na6 -14.0(10) . . . 1_565 ?
O29 W9 O31 Na6 -101.2(9) . . . 1_565 ?
O3 W9 O31 Na6 -56.9(17) . . . 1_565 ?
O25 W7 O32 W10 -142.6(4) . . . 2_556 ?
O26 W7 O32 W10 114.6(4) . . . 2_556 ?
O24 W7 O32 W10 -47.2(4) . . . 2_556 ?
O14 W7 O32 W10 26.9(10) . . . 2_556 ?
O2 W7 O32 W10 26.6(4) . . . 2_556 ?
O25 W7 O32 Zn2 -142.6(4) . . . 2_556 ?
O26 W7 O32 Zn2 114.6(4) . . . 2_556 ?
O24 W7 O32 Zn2 -47.2(4) . . . 2_556 ?
O14 W7 O32 Zn2 26.9(10) . . . 2_556 ?
O2 W7 O32 Zn2 26.6(4) . . . 2_556 ?
O25 W7 O32 Zn3 61.3(3) . . . 2_556 ?
O26 W7 O32 Zn3 -41.4(3) . . . 2_556 ?
O24 W7 O32 Zn3 156.7(3) . . . 2_556 ?
O14 W7 O32 Zn3 -129.2(6) . . . 2_556 ?
O2 W7 O32 Zn3 -129.5(3) . . . 2_556 ?

_refine_diff_density_max         2.145
_refine_diff_density_min         -2.245
_refine_diff_density_rms         0.338

_shelxl_version_number           2013-4


_exptl_crystal_recrystallization_method 'Re-crystallisation from solvent: water'
